This thesis is divided into 8 chapters.
The first (current) introduction chapter includes the basics of InGaAs as a semiconductor material, a brief review of ternary III-V nanowires and introduces the global aims of this thesis. This chapter also highlights the areas which require attention which could be enhanced further to improve our knowledge in understanding the growth mechanism of ternary alloy nanowires, especially InGaAs nanowires which has great potential in high- speed telecommunication and near infra-red application.
Chapter 2 discusses the basic concepts of semiconductor nanowires, growth of nanowires and their heterostructures and their crystallographic structural properties.
Chapter 3 describes the experimental technique used in this study. The first section in this chapter explains the growth method used for growing InGaAs nanowires including the wafer preparation and MOVPE. The following 4 sections in the chapter briefly discussthe techniques used to characterise the nanowires including electron microscopy and photoluminescence technique.
In chapter 4, the results obtained via two-temperature growth method are discussed. Although the two-temperature growth technique has been a great a success to synthesise high quality GaAs nanowires, it is more challenging in growing ternary InGaAs nanowires which results in further complexity. This chapter discusses the effect of growth temperature, precursor ratios and vapour composition. Albeit challenging, successful InGaAs nanowires with pure ZB phase could be achieved for high In content (In0.95Ga0.05As).
Such nanowires are useful to replace InAs nanowires as they have lower leakage current due to the larger bandgap with the introduction of Ga. Hence, it is highly important to be able to grow such structures with highly pure crystal phase in order to realise fast-switching devices which require high electron mobility.
In chapter 5, growth of InGaAs nanowires aiming at a uniform pure WZ crystal structure and high compositional homogeneity is presented. V/III ratio is shown to have control over the tunability of InGaAs composition and crystal phase. The key factors for achieving uniform composition are summarised. In0.65Ga0.35As nanowires are shown to grow
with negligible tapering, uniform composition and were shown to have strong emission at the desirable wavelength for telecommunications applications around 1.55 µm when capped with an InP shell.
A growth model is then proposed and developed to further understand the growth trend observed as detailed in chapter 6. The main factors affecting the axial growth rate and the composition of InGaAs nanowires are extracted based on correlation of the model to the experimental results. The model provides a better understanding on the growth of InGaAs nanowires.
Chapter 7 shows and discusses the results of InGaAs/InGaP core-shell heterostructures. It explores tuning of the bandgap of the InGaAs core using various shell thickness. The chapter also discusses the growth of InGaP shell on WZ phase InGaAs and ZB InGaAs nanowires. The bandgap of InGaAs nanowires is shown to be tunable using InGaP shell with various shell thicknesses.
Finally, conclusions and future work are provided in chapter 8 discussing the outcomes achieved from the thesis and potential research extension that can be followed to develop more knowledge and potential devices based on ternary and quaternary alloy nanowires.
 R. S. Wagner and W. C. Ellis, “Vapor-liquid-solid mechanism of single crystal growth,”
Appl. Phys. Lett., vol. 4, no. 5, pp. 89–90, 1964.
 E. I. Givargizov, “Fundamental aspects of VLS growth,” J. Cryst. Growth, vol. 31, pp. 20– 30, 1975.
 K. A. Dick, “A review of nanowire growth promoted by alloys and non-alloying
elements with emphasis on Au-assisted III-V nanowires,” Prog. Cryst. Growth Charact. Mater., vol. 54, no. 3–4, pp. 138–173, 2008.
 S. A. Fortuna and X. Li, “Metal-catalyzed semiconductor nanowires: a review on the control of growth directions,” Semicond. Sci. Technol., vol. 25, no. 2, p. 024005, 2010.  R. R. Lapierre, A. C. E. Chia, S. J. Gibson, C. M. Haapamaki, J. Boulanger, R. Yee, P.
Kuyanov, J. Zhang, N. Tajik, N. Jewell, and K. M. A. Rahman, “III-V nanowire
photovoltaics: Review of design for high efficiency,” Phys. Status Solidi - Rapid Res. Lett., vol. 7, no. 10, pp. 815–830, 2013.
 L. Vj, J. Oh, A. P. Nayak, A. M. Katzenmeyer, K. Gilchrist, S. Grego, N. P. Kobayashi, S. Wang, A. A. Talin, N. K. Dhar, and M. M. Islam, “A Perspective on Nanowire
Photodetectors: Current Status, Future Challenges, and Opportunities,” Sel. Top. Quantum Electron. IEEE J., vol. PP, no. 99, pp. 1–31, 2011.
 C. Soci, A. Zhang, X.-Y. Bao, H. Kim, Y. Lo, and D. Wang, “Nanowire photodetectors.,” J. Nanosci. Nanotechnol., vol. 10, no. 3, pp. 1430–1449, 2010.
 E. C. Garnett, M. L. Brongersma, Y. Cui, and M. D. McGehee, “Nanowire Solar Cells,”
Annu. Rev. Mater. Res., vol. 41, no. 1, pp. 269–295, 2011.
 S. Barth, F. Hernandez-Ramirez, J. D. Holmes, and A. Romano-Rodriguez, “Synthesis and applications of one-dimensional semiconductors,” Prog. Mater. Sci., vol. 55, no. 6, pp. 563–627, 2010.
 X. Zhuang, C. Z. Ning, and A. Pan, “Composition and bandgap-graded semiconductor alloy nanowires,” Adv. Mater., vol. 24, no. 1, pp. 13–33, 2012.
 L.-E. Wernersson, C. Thelander, E. Lind, and L. Samuelson, “III-V Nanowires - Extending a Narrowing Road,” Proc. IEEE, vol. 98, no. 12, pp. 2047–2060, 2010.  A. Rogalski and K. Chrzanowski, “Infrared devices and techniques,” Optoelectron. Rev.,
vol. 10, no. 2, pp. 653–691, 2002.
 R. E. Nahory, M. A. Pollack, W. D. Johnston, and R. L. Barns, “Band gap versus
composition and demonstration of Vegard’s law for In1−xGaxAsyP1−y lattice matched to
InP,” Appl. Phys. Lett., vol. 33, no. 7, p. 659, Aug. 1978.
 Y. Li, F. Qian, J. Xiang, and C. M. Lieber, “Nanowire electronic and optoelectronic devices Electronic and optoelectronic devices impact many areas of society , from,”
Mater. Today, vol. 9, no. 10, pp. 18–27, 2006.
 H. J. Joyce, Q. Gao, H. Hoe Tan, C. Jagadish, Y. Kim, J. Zou, L. M. Smith, H. E. Jackson, J. M. Yarrison-Rice, P. Parkinson, and M. B. Johnston, “III-V semiconductor nanowires for optoelectronic device applications,” Prog. Quantum Electron., vol. 35, no. 2–3, pp. 23– 75, 2011.
 J. W. Harrison and J. R. Hauser, “Alloy scattering in ternary III-V compounds,” Phys. Rev. B, vol. 13, no. 12, 1976.
 M. Ichimura and A. Sasaki, “Short-range order in III-V ternary alloy semiconductors,”
J. Appl. Phys., vol. 60, no. 11, pp. 3850–3855, 1986.
 P. Caroff, M. E. Messing, B. Mattias Borg, K. A. Dick, K. Deppert, and L.-E. Wernersson, “InSb heterostructure nanowires: MOVPE growth under extreme lattice mismatch.,”
Nanotechnology, vol. 20, no. 49, p. 495606, 2009.
 H. D. Park, S. M. Prokes, M. E. Twigg, Y. Ding, and Z. L. Wang, “Growth of high quality, epitaxial InSb nanowires,” J. Cryst. Growth, vol. 304, no. 2, pp. 399–401, Jun. 2007.  K. A. Dick, K. Deppert, L. Samuelson, L. R. Wallenberg, and F. M. Ross, “Control of GaP
and GaAs nanowire morphology through particle and substrate chemical modification,” Nano Lett., vol. 8, no. 11, pp. 4087–4091, 2008.
 H. J. Joyce, Q. Gao, J. Wong-Leung, Y. Kim, H. H. Tan, and C. Jagadish, “Tailoring GaAs, InAs, and InGaAs nanowires for optoelectronic device applications,” IEEE J. Sel. Top. Quantum Electron., vol. 17, no. 4, pp. 766–778, 2011.
 K. A. Dick, J. Bolinsson, M. E. Messing, S. Lehmann, J. Johansson, and P. Caroff,
“Parameter space mapping of InAs nanowire crystal structure,” J. Vac. Sci. Technol. B Microelectron. Nanom. Struct., vol. 29, no. 4, p. 04D103, 2011.
 K. A. Dick, K. Deppert, L. Samuelson, and W. Seifert, “Optimization of Au-assisted InAs nanowires grown by MOVPE,” J. Cryst. Growth, vol. 297, no. 2, pp. 326–333, 2006.  K. A. Dick, P. Caroff, J. Bolinsson, M. E. Messing, J. Johansson, K. Deppert, L. R.
Wallenberg, and L. Samuelson, “Control of III–V nanowire crystal structure by growth parameter tuning,” Semicond. Sci. Technol., vol. 25, no. 2, p. 024009, Feb. 2010.
 C. C. Chen and C. C. Yeh, “Large-scale catalytic synthesis of crystalline gallium nitride nanowires,” Adv. Mater., vol. 12, no. 10, pp. 738–741, 2000.
 K. W. Chang and J. J. Wu, “Low-temperature catalytic synthesis of gallium nitride nanowires,” J. Phys. Chem. B, vol. 106, no. 32, pp. 7796–7799, 2002.
 X. Duan and C. M. Lieber, “General synthesis of compound semiconductor nanowires,”
 T. Kuykendall, P. Ulrich, S. Aloni, and P. Yang, “Complete composition tunability of InGaN nanowires using a combinatorial approach.,” Nat. Mater., vol. 6, no. 12, pp. 951–956, 2007.
 J. Su, M. Gherasimova, G. Cui, H. Tsukamoto, J. Han, T. Onuma, M. Kurimoto, S. F. Chichibu, C. Broadbridge, Y. He, and A. V. Nurmikko, “Growth of AlGaN nanowires by metalorganic chemical vapor deposition,” Appl. Phys. Lett., vol. 87, no. 18, pp. 1–3, 2005.
 C. Chen, S. Shehata, C. Fradin, R. LaPierre, C. Couteau, and G. Weihs, “Self-directed growth of AlGaAs core-shell nanowires for visible light applications,” Nano Lett., vol. 7, no. 9, pp. 2584–2589, 2007.
 Z. H. Wu, M. Sun, X. Y. Mei, and H. E. Ruda, “Growth and photoluminescence characteristics of AlGaAs nanowires,” Appl. Phys. Lett., vol. 85, no. 4, pp. 657–659, 2004.
 Y. Kim, H. J. Joyce, Q. Gao, H. H. Tan, C. Jagadish, M. Paladugu, J. Zou, and A. A. Suvorova, “Influence of nanowire density on the shape and optical properties of ternary InGaAs nanowires,” Nano Lett., vol. 6, no. 4, pp. 599–604, 2006.
 S. K. Lim, M. J. Tambe, M. M. Brewster, and S. Gradecak, “Controlled growth of ternary alloy nanowires using metalorganic chemical vapor deposition.,” Nano Lett., vol. 8, no. 5, pp. 1386–1392, 2008.
 A. Fakhr, Y. M. Haddara, and R. R. Lapierre, “Dependence of InGaP nanowire morphology and structure on molecular beam epitaxy growth conditions.,”
Nanotechnology, vol. 21, no. 16, p. 165601, 2010.
 Y. N. Guo, H. Y. Xu, G. J. Auchterlonie, T. Burgess, H. J. Joyce, Q. Gao, H. H. Tan, C. Jagadish, H. B. Shu, X. S. Chen, W. Lu, Y. Kim, and J. Zou, “Phase separation induced by Au catalysts in ternary InGaAs nanowires,” Nano Lett., vol. 13, no. 2, pp. 643–650, 2013.
 W. Sun, Y. Huang, Y. Guo, Z. M. Liao, Q. Gao, H. H. Tan, C. Jagadish, X. Z. Liao, and J. Zou, “Spontaneous formation of core–shell GaAsP nanowires and their enhanced electrical conductivity,” J. Mater. Chem. C, vol. 3, no. 8, pp. 1745–1750, 2015.
 J. Wu, B. M. Borg, D. Jacobsson, K. A. Dick, and L. E. Wernersson, “Control of composition and morphology in InGaAs nanowires grown by metalorganic vapor phase epitaxy,” J. Cryst. Growth, vol. 383, pp. 158–165, 2013.
 C. Thelander, P. Caroff, S. Plissard, A. W. Dey, and K. A. Dick, “Effects of crystal phase mixing on the electrical properties of InAs nanowires,” Nano Lett., vol. 11, no. 6, pp. 2424–2429, 2011.
 P. J. Poole, D. Dalacu, X. Wu, J. Lapointe, and K. Mnaymneh, “Interplay between crystal phase purity and radial growth in InP nanowires,” Nanotechnology, vol. 23, no. 38, p. 385205, 2012.
 M. Heiss, B. Ketterer, E. Uccelli, J. R. Morante, J. Arbiol, and A. Fontcuberta i Morral, “In(Ga)As quantum dot formation on group-III assisted catalyst-free InGaAs nanowires.,” Nanotechnology, vol. 22, no. 19, p. 195601, 2011.
 Y. Y. Zhang, M. Aagesen, J. V Holm, H. I. Jorgensen, J. Wu, and H. Y. Liu, “Self-Catalyzed GaAsP Nanowires Grown on Silicon Substrates by Solid-Source Molecular Beam Epitaxy,” Nano Lett., vol. 13, pp. 3897–3902, 2013.
 T. Xu, K. A. Dick, S. Plissard, T. H. Nguyen, Y. Makoudi, M. Berthe, J.-P. Nys, X. Wallart, B. Grandidier, and P. Caroff, “Faceting, composition and crystal phase evolution in III– V antimonide nanowire heterostructures revealed by combining microscopy
techniques,” Nanotechnology, vol. 23, no. 9, p. 095702, 2012.
 M. Heiss, A. Gustafsson, S. Conesa-Boj, F. Peiró, J. R. Morante, G. Abstreiter, J. Arbiol, L. Samuelson, and A. Fontcuberta i Morral, “Catalyst-free nanowires with axial InxGa1- xAs/GaAs heterostructures.,” Nanotechnology, vol. 20, no. 7, p. 075603, 2009.  J. Paek, M. Yamaguchi, and H. Amano, “MBE-VLS growth of catalyst-free III-V axial
heterostructure nanowires on (1 1 1)Si substrates,” J. Cryst. Growth, vol. 323, no. 1, pp. 315–318, 2011.
 S. G. Ghalamestani, M. Ek, M. Ghasemi, P. Caroff, J. Johansson, and K. A. Dick, “Morphology and composition controlled GaxIn1-xSb nanowires: understanding
ternary antimonide growth.,” Nanoscale, vol. 6, no. 2, pp. 1086–92, 2014.  J. Bauer, V. Gottschalch, H. Paetzelt, and G. Wagner, “VLS growth of
GaAs/(InGa)As/GaAs axial double-heterostructure nanowires by MOVPE,” J. Cryst. Growth, vol. 310, no. 23, pp. 5106–5110, 2008.
 C. S. Jung, H. S. Kim, G. B. Jung, K. J. Gong, Y. J. Cho, S. Y. Jang, C. H. Kim, C. W. Lee, and J. Park, “Composition and phase tuned InGaAs alloy nanowires,” J. Phys. Chem. C, vol. 115, no. 16, pp. 7843–7850, 2011.
 H. S. Im, C. S. Jung, K. Park, D. M. Jang, Y. R. Lim, and J. Park, “Band gap tuning of twinned GaAsP ternary nanowires,” J. Phys. Chem. C, vol. 118, no. 8, pp. 4546–4552, 2014.
 S. Conesa-Boj, D. Kriegner, X. L. Han, S. Plissard, X. Wallart, J. Stangl, A. Fontcuberta I Morral, and P. Caroff, “Gold-free ternary III-V antimonide nanowire arrays on silicon: Twin-free down to the first bilayer,” Nano Lett., vol. 14, no. 1, pp. 326–332, 2014.  X. Yuan, P. Caroff, J. Wong-Leung, H. H. Tan, and C. Jagadish, “Controlling the
morphology, composition and crystal structure in gold-seeded GaAs 1−x Sb x nanowires,” Nanoscale, vol. 7, no. 11, pp. 4995–5003, 2015.
 Y. N. Guo, T. Burgess, Q. Gao, H. H. Tan, C. Jagadish, and J. Zou, “Polarity-driven nonuniform composition in InGaAs nanowires,” Nano Lett., vol. 13, no. 11, pp. 5085– 5089, 2013.
 N. Sköld, J. B. Wagner, G. Karlsson, T. Hernán, W. Seifert, M.-E. Pistol, and L.
Samuelson, “Phase segregation in AlInP shells on GaAs nanowires.,” Nano Lett., vol. 6, no. 12, pp. 2743–2747, 2006.
 J. B. Wagner, N. Sköld, L. Reine Wallenberg, and L. Samuelson, “Growth and
segregation of GaAs-AlxIn1-xP core-shell nanowires,” J. Cryst. Growth, vol. 312, no. 10, pp. 1755–1760, 2010.
 N. Jiang, Q. Gao, P. Parkinson, J. Wong-Leung, S. Mokkapati, S. Breuer, H. H. Tan, C. L. Zheng, J. Etheridge, and C. Jagadish, “Enhanced minority carrier lifetimes in
GaAs/AlGaAs core-shell nanowires through shell growth optimization,” Nano Lett., vol. 13, no. 11, pp. 5135–5140, 2013.
 M. Fickenscher, T. Shi, H. E. Jackson, L. M. Smith, J. M. Yarrison-rice, C. Zheng, P. Miller, J. Etheridge, B. M. Wong, Q. Gao, S. Deshpande, H. H. Tan, and C. Jagadish, “Optical , Structural , and Numerical Investigations of GaAs / AlGaAs Core − Multishell Nanowire Quantum Well Tubes,” 2013.
 D. Rudolph, S. Funk, M. Döblinger, S. Morkötter, S. Hertenberger, L. Schweickert, J. Becker, S. Matich, M. Bichler, D. Spirkoska, I. Zardo, J. J. Finley, G. Abstreiter, and G. Koblmüller, “Spontaneous alloy composition ordering in GaAs-AlGaAs core-shell nanowires,” Nano Lett., vol. 13, no. 4, pp. 1522–1527, 2013.
 H. Kauko, C. L. Zheng, Y. Zhu, S. Glanvill, C. Dwyer, A. M. Munshi, B. O. Fimland, A. T. J. Van Helvoort, and J. Etheridge, “Compositional analysis of GaAs/AlGaAs
heterostructures using quantitative scanning transmission electron microscopy,”
Appl. Phys. Lett., vol. 103, no. 23, 2013.
 Y. Zhang, A. M. Sanchez, J. Wu, M. Aagesen, J. V. Holm, R. Beanland, T. Ward, and H. Liu, “Polarity-Driven Quasi-3-Fold Composition Symmetry of Self-Catalyzed III–V–V Ternary Core–Shell Nanowires,” Nano Lett., vol. 15, pp. 3128–3133, 2015.  M. Heiss, Y. Fontana, A. Gustafsson, G. Wüst, C. Magen, D. D. O’Regan, J. W. Luo, B.
Ketterer, S. Conesa-Boj, A. V Kuhlmann, J. Houel, E. Russo-Averchi, J. R. Morante, M. Cantoni, N. Marzari, J. Arbiol, A. Zunger, R. J. Warburton, and A. Fontcuberta i Morral, “Self-assembled quantum dots in a nanowire system for quantum photonics.,” Nat. Mater., vol. 12, no. 5, pp. 439–44, 2013.
 J. C. Shin, K. H. Kim, K. J. Yu, H. Hu, L. Yin, C. Ning, J. a Rogers, J. Zuo, and X. Li, “In
xGa1 - xAs Nanowires on Silicon : One-Dimensional Heterogeneous epitaxy, bandgap
engineering and photovotaic,” Nano Lett., vol. 11, pp. 4831–4838, 2011.
 K. W. Ng, W. S. Ko, F. Lu, and C. J. Chang-Hasnain, “Metastable growth of pure wurtzite InGaAs microstructures,” Nano Lett., vol. 14, no. 8, pp. 4757–4762, 2014.
 K. W. Ng, W. S. Ko, R. Chen, F. Lu, T. D. Tran, K. Li, and C. J. Chang-Hasnain,
“Composition Homogeneity in InGaAs/GaAs Core − Shell Nanopillars Monolithically Grown on Silicon,” Appl. Mater. Interfaces, vol. 6, no. 19, pp. 16706–11, 2014.
 P. K. Mohseni, A. Behnam, J. D. Wood, C. D. English, J. W. Lyding, E. Pop, and X. Li, “InxGa1-xAs Nanowire Growth on Graphene: van der Waals Epitaxy Induced Phase
Segregation,” Nano Lett., vol. 13, pp. 1153–1161, 2013.
 Y. Kohashi, T. Sato, K. Ikejiri, K. Tomioka, S. Hara, and J. Motohisa, “Influence of growth temperature on growth of InGaAs nanowires in selective-area metalorganic vapor-phase epitaxy,” J. Cryst. Growth, vol. 338, no. 1, pp. 47–51, 2012.
 T. Sato, Y. Kobayashi, J. Motohisa, S. Hara, and T. Fukui, “SA-MOVPE of InGaAs nanowires and their compositions studied by micro-PL measurement,” J. Cryst. Growth, vol. 310, no. 23, pp. 5111–5113, 2008.
 T. Sato, J. Motohisa, J. Noborisaka, S. Hara, and T. Fukui, “Growth of InGaAs nanowires by selective-area metalorganic vapor phase epitaxy,” J. Cryst. Growth, vol. 310, no. 7– 9, pp. 2359–2364, 2008.
 M. Yoshimura, K. Tomioka, K. Hiruma, S. Hara, J. Motohisa, and T. Fukui, “Growth and characterization of InGaAs nanowires formed on GaAs(111)B by selective-area metal organic vapor phase epitaxy,” Jpn. J. Appl. Phys., vol. 49, no. 4 PART 2, pp. 8–12, 2010.  S. Hertenberger, S. Funk, K. Vizbaras, a. Yadav, D. Rudolph, J. Becker, S. Bolte, M.
Döblinger, M. Bichler, G. Scarpa, P. Lugli, I. Zardo, J. J. Finley, M. C. Amann, G. Abstreiter, and G. Koblmüller, “High compositional homogeneity in In-rich InGaAs nanowire arrays on nanoimprinted SiO 2/Si (111),” Appl. Phys. Lett., vol. 101, no. 4, 2012.
 G. Koblmuller and G. Abstreiter, “Growth and properties of InGaAs nanowires on silicon,” Phys. Status Solidi RRL, vol. 7, no. 10, pp. 1–20, 2014.
 H. Sun, F. Ren, K. W. Ng, T. T. D. Tran, K. Li, and C. J. Chang-Hasnain, “Nanopillar lasers directly grown on silicon with heterostructure surface passivation,” ACS Nano, vol. 8, no. 7, pp. 6833–6839, 2014.
 J. V Holm, H. I. Jørgensen, P. Krogstrup, J. Nygård, H. Liu, and M. Aagesen, “Surface- passivated GaAsP single-nanowire solar cells exceeding 10% efficiency grown on silicon.,” Nat. Commun., vol. 4, p. 1498, 2013.
 T. Yang, S. Hertenberger, S. Morkötter, G. Abstreiter, and G. Koblmüller, “Size, composition, and doping effects on In(Ga)As nanowire/Si tunnel diodes probed by conductive atomic force microscopy,” Appl. Phys. Lett., vol. 101, no. 23, pp. 233102–1– 5, 2012.
 J. J. Hou, N. Han, F. Wang, F. Xiu, S. Yip, A. T. Hui, T. Hung, and J. C. Ho, “Synthesis and characterizations of ternary InGaAs nanowires by a two-step growth method for high-performance electronic devices,” ACS Nano, vol. 6, no. 4, pp. 3624–3630, 2012.  K. Tomioka, M. Yoshimura, and T. Fukui, “A III–V nanowire channel on silicon for
high-performance vertical transistors,” Nature, vol. 488, no. 7410, pp. 189–192, 2012.  M. N. Makhonin, a. P. Foster, a. B. Krysa, P. W. Fry, D. G. Davies, T. Grange, T. Walther,
M. S. Skolnick, and L. R. Wilson, “Homogeneous array of nanowire-embedded quantum light emitters,” Nano Lett., vol. 13, no. 3, pp. 861–865, 2013.
 F. Qian, Y. Li, S. Gradecak, H.-G. Park, Y. Dong, Y. Ding, Z. L. Wang, and C. M. Lieber,